Significance and Use
This test method may be used for material development, material comparison, quality assurance, characterization, and design data generation.
Continuous fiber-reinforced ceramic matrix composites are candidate materials for structural applications requiring high degrees of wear and corrosion resistance and toughness at high temperatures.
Creep tests measure the time-dependent deformation of a material under constant load at a given temperature. Creep rupture tests provide a measure of the life of the material when subjected to constant mechanical loading at elevated temperatures. In selecting materials and designing parts for service at elevated temperatures, the type of test data used will depend on the criteria for load-carrying capability which best defines the service usefulness of the material.
Creep and creep rupture tests provide information on the time-dependent deformation and on the time-of-failure of materials subjected to uniaxial tensile stresses at elevated temperatures. Uniform stress states are required to effectively evaluate any nonlinear stress-strain behavior which may develop as the result of cumulative damage processes (for example, matrix cracking, matrix/fiber debonding, fiber fracture, delamination, etc.) which may be influenced by testing mode, testing rate, processing or alloying effects, environmental influences, or elevated temperatures. Some of these effects may be consequences of stress corrosion or subcritical (slow) crack growth. It is noted that ceramic materials typically creep more rapidly in tension than in compression. Therefore, creep data for design and life prediction should be obtained in both tension and compression.
The results of tensile creep and tensile creep rupture tests of specimens fabricated to standardized dimensions from a particular material or selected portions of a part, or both, may not totally represent the creep deformation and creep rupture properties of the entire, full-size end product or its in-service behavior in different environments or at various elevated temperatures.
For quality control purposes, results derived from standardized tensile test specimens may be considered indicative of the response of the material from which they were taken for given primary processing conditions and post-processing heat treatments.
1.1 This test method covers the determination of the time-dependent deformation and time-to-rupture of continuous fiber-reinforced ceramic composites under constant tensile loading at elevated temperatures. This test method addresses, but is not restricted to, various suggested test specimen geometries. In addition, test specimen fabrication methods, allowable bending, temperature measurements, temperature control, data collection, and reporting procedures are addressed.
1.2 This test method is intended primarily for use with all advanced ceramic matrix composites with continuous fiber reinforcement: unidirectional (1-D), bidirectional (2-D), and tridirectional (3-D). In addition, this test method may also be used with glass matrix composites with 1-D, 2-D, and 3-D continuous fiber reinforcement. This test method does not address directly discontinuous fiber-reinforced, whisker-reinforced, or particulate-reinforced ceramics, although the test methods detailed here may be equally applicable to these composites.
1.3 Values expressed in this test method are in accordance with the International System of Units (SI) and .
1.4 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use. Hazard statements are noted in 7.1 and 7.2.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
C1145 Terminology of Advanced Ceramics
C1275 Test Method for Monotonic Tensile Behavior of Continuous Fiber-Reinforced Advanced Ceramics with Solid Rectangular Cross-Section Test Specimens at Ambient Temperature
D3878 Terminology for Composite Materials
E4 Practices for Force Verification of Testing Machines
E6 Terminology Relating to Methods of Mechanical Testing
E83 Practice for Verification and Classification of Extensometer Systems
E139 Test Methods for Conducting Creep, Creep-Rupture, and Stress-Rupture Tests of Metallic Materials
E220 Test Method for Calibration of Thermocouples By Comparison Techniques
E230 Specification and Temperature-Electromotive Force (EMF) Tables for Standardized Thermocouples
E337 Test Method for Measuring Humidity with a Psychrometer (the Measurement of Wet- and Dry-Bulb Temperatures)
E1012 Practice for Verification of Testing Frame and Specimen Alignment Under Tensile and Compressive Axial Force Application
ceramic matrix composite; CFCC; continuous fiber ceramic composite; creep rupture; creep test; elevated temperature; Ceramic composites; Composites; Continuous fiber-reinforced ceramic composites (CFCC); Creep; Creep rupture; Elevated temperature tests; Fiber-reinforced composites; Tensile loading;
ICS Number Code 19.060 (Mechanical testing); 81.060.99 (Other standards related to ceramics); 81.060.30 (Advanced ceramics)
ASTM International is a member of CrossRef.
Citing ASTM Standards
[Back to Top]